http://www.scirp.org/journal/msce ISSN Online: 2327-6053 ISSN Print: 2327-6045
DOI: 10.4236/msce.2017.511004 Nov. 17, 2017 33 Journal of Materials Science and Chemical Engineering
Effect of High Temperatures on the
Microstructure of Cement Paste
M. A. Tantawy
Chemistry Department, Faculty of Science, Minia University, Minya, Egypt
The microstructural and compositional changes within the cement paste ex-posed to high temperatures were monitored by XRD, FTIR, TGA/DTA and SEM techniques to understand the nature of decomposition of C-S-H gel and the associated physicomechanical properties of thermally damaged cement paste. OPC paste (w/c ratio 0.27) was hydrated for 28 days then fired up to 750˚C for 2 hours (heating rate 10˚C/min). The relative mass percent of cal-cium hydrates and portlandite was estimated by calculations derived from TGA results. Beyond 450˚C, the percentage of portlandite sharply diminishes and C-S-H progressively decomposes into C2S and C3S until complete loss of calcium hydrates content occurs at 750˚C. An increase of the total porosity, severe loss in mechanical strength and propagation of harmful cracks occurs. The thermal shock as a result of cooling of the heated cement paste and the rehydration of lime enhance the propagation of harmful cracks.
Cement paste, C-S-H, Portlandite, Dehydration, Microstructure
The exposure of concrete to high temperatures induces severe microstructural changes and concrete loses its strength and durability . Concrete approx-imately loses half of its strength at a temperature of 600˚C and loses most of its compressive strength above 800˚C . The literature that deals with the effect of high temperatures on the properties of concrete can be divided into two catego-ries. The first category investigates the degree of deterioration on the mechanical properties of concrete exposed to high temperatures and evaluates the fire dam-aged concrete by using nondestructive tools such as ultrasonic and resonance vibration techniques . The influence of high temperatures on the
mechan-How to cite this paper: Tantawy, M.A. (2017) Effect of High Temperatures on the Microstructure of Cement Paste. Journal of Materials Science and Chemical Engineer-ing, 5, 33-48.
Received: September 11, 2017 Accepted: November 14, 2017 Published: November 17, 2017 Copyright © 2017 by author and Scientific Research Publishing Inc. This work is licensed under the Creative Commons Attribution International License (CC BY 4.0).
DOI: 10.4236/msce.2017.511004 34 Journal of Materials Science and Chemical Engineering ical properties of concrete depends on physico-chemical properties of the con-crete constituents  , temperature of exposure , size of the concrete structure , external applied loadings  and cooling conditions . The second category investigates the microstructural changes induced in concrete exposed to high temperatures.
The deterioration of concrete exposed to high temperatures is attributed to: 1) The thermal mismatch due to the expansion of siliceous aggregate and shrinkage of cement paste matrix ,
2) The decomposition of hydrates due to the decomposition of portlandite and C-S-H ,
3) The coarsening of pore structure due to void formation as a result of loss of bound water ,
4) The pore pressure effects due to buildup of vapor pressure inside closed pores  and,
5) Cracking that develops as a result of the rehydration of lime .
In literature, the following investigations were performed on cement paste af-ter exposure to high temperatures.
1) Assessment of the structural properties of cement paste such as stiffness of cement paste by absorption capacity , pore structure by backscattered elec-tron microscopy/mercury intrusion porosimetry/gas permeability techniques , and crack density by digital microscope .
2) Evaluation of the microstructural changes by XRD, DSC/TGA/DTG/DTA and SEM/EDX techniques -.
3) Monitoring of the phase transformations by instrumental techniques  .
4) Estimation of the cementitious phases  .
5) Estimation of the dehydration mechanisms and kinetics for decomposition of portlandite and C-S-H .
The major changes that occur within cement paste due to exposure to high temperatures include the decomposition of portlandite and calcium silicate hy-drates . There is a contradiction in the literature about the nature and types of the decomposition products of C-S-H gel which decomposes over a wide range temperature (about from 105˚C to 1000˚C ) as a result of its amorph-ous nature. Zhang and Ye calculated the activation energy (Ea) of the dehydra-tion of C-S-H and portlandite by Arrhenius equadehydra-tion from TGA/DTG results. Eaportlandite is about 151.82 kJ/mol whereas EaC-S-H varies from 83.69 to 371.93 kJ/mol. Accordingly, the dehydration of portlandite is a single-step reaction, whereas the dehydration of C-S-H is a multi-step reaction because of its complex structure .
DOI: 10.4236/msce.2017.511004 35 Journal of Materials Science and Chemical Engineering temperature range of 110˚C - 450˚C and transforms to C2S and C3S above 600˚C . According to Heikal, C-S-H gel dehydrates in the temperature range of 100˚C - 400˚C and transforms to C2S and C3S at 800˚C . According to Peng, C-S-H gel started to decompose at 560˚C and transforms to C2S and C3S at 800˚C .
According to Ghosh et al., the rehydration of dehydrated phases that take place in the fired cement pastes after cooling at moist air, that together with the changes in volume, and mass may lead to an additional increase in the porosity of cement paste and enhances the formation of additional cracks . Many re-searchers reported that there are many factors that control the extent of deteri-oration caused by CaO rehydration such as the rate of water absorption  and the initial mineralogy of Portland cement, (i.e. primarily the amount alumina phases ). The estimation of rehydrating portlandite can be used as tracers for determining the heating history of concrete exposed to high temperatures . Many researchers investigated the effect of high temperatures and rehydration on the mechanical properties of blended cement pastes. According to Vysvaril et al., the cement paste with the addition of granulated blast furnace slag has the best resistivity to high temperatures; however, the limestone cement paste shows better mechanical properties after rehydration process . In contrast, the re-hydration process promotes the reformation of C-S-H gel from the nesosilicate phase as well as the recrystallization of calcite, portlandite and ettringite phases . In the other hand, it was reported that the rehydration of the anhydrous phases is accompanied by partial recovery of the mechanical properties of the fire-exposed concrete structure  and . The rehydration process displays cementitious behavior similar to that of the calcium silicates present in Portland cement, developing strength and thus potentially enabling the production of construction materials. According to Shui et al., the addition of fly ash and Port-land cement to preheated recycled concrete can significantly enhance its rehy-drated strength . Serpell and Lopez developed reactivated cementitious ma-terials from recycling of hydrated cement paste wastes as alternative binders of high environmental value .
The aim of this contribution is to monitor the microstructure and phase changes of cement paste exposed to high temperatures up to 750˚C by XRD, FTIR, TGA/DTA and SEM techniques and to correlate the phase changes with the physico-mechanical properties of the thermally damaged cement paste. What differentiate this work from that of others is that the approximate percen-tage of residual calcium hydrates (C-S-H, ettringite and calcium aluminate hy-drates) in cement pastes fired at a given temperature relative to that in unfired cement paste was estimated.
2. Materials and Experimental Techniques
DOI: 10.4236/msce.2017.511004 36 Journal of Materials Science and Chemical Engineering under water to enhance hydration of the cement paste before being subjected to the fire experiment. The compressive strength of the cement pastes was meas-ured using a manual compressive strength machine according to ASTM desig-nation .
The loss in compressive strength (L) was calculated according to :
L= −l S S ×
where Sf is the compressive strength after exposure to high temperature, and S is the compressive strength before exposure to high temperature.
Termination of the hydration of cement paste was performed using a domes-tic microwave oven . The bulk density of unfired cement pastes was meas-ured according to the Archimedes principle . Bulk density was determined as the weight of the cement paste divided by its volume. Where the volume of cement paste is calculated from the weight difference between cement in air and suspended in water. Each measurement was carried out on three similar speci-mens of the same testing time. The total porosity of unfired cement pastes was measured as described elsewhere . The total porosity was calculated from the values of bulk density as well as the free and total water contents of the cement paste. Cement pastes were dried at 105˚C for 24 hours and fired at 300˚C, 450˚C, 600˚C and 750˚C for 2 hours in a muffle furnace with a heating rate of 10˚C/min. The heating curve was illustrated Figure 1. The desired temperature was maintained for 2 hours. At the end of the heating period, the specimens were removed from the furnace and were cooled down to room temperature in a desiccator. The weight loss of fired cement pastes was measured as the percen-tage of the weight loss based on weight after firing. The bulk density and total porosity of fired cement pastes were measured according to the ISO 5018-1983 . XRF analysis was performed by Philips PW 1606 x-ray fluorescence spec-trometer. XRD analysis was performed by Philips x-ray diffractometer PW 1370 with Ni filtered CuKα radiation (1.5406 Å). The semi-quantitative phase deter-mination was estimated by measuring the areas of representative peaks, using X’Pert HighScore Plus software and JCPDS-ICDD data base. The standard devi-ation was ±5%. FTIR analysis was performed by spectrometer Perkin Elmer FTIR System Spectrum X in the range 400 - 4000 cm−1. SEM analysis was per-formed by Jeol-Dsm 5400 LG apparatus. TGA/DrTGA/DTA were perper-formed by Shimadzu Corporation thermo analyzer with DTG-60H detector with 10˚C/min heating rate from the room temperature up to 1000˚C, under air
Figure 1. The muffle furnace and heating profile.
Heating rate = 10˚C/min Cooling rate >> 10˚C/min
DOI: 10.4236/msce.2017.511004 37 Journal of Materials Science and Chemical Engineering atmosphere at 40 ml/min flow rate, the hold time at the appropriate temperature is zero.
The percentage of portlandite (P) in the unfired and fired cement pastes was calculated for the following reaction (Ca(OH)2 → CaO + H2O) as :
P= ⋅ ∆f wt
where; F is the mole ratio Ca(OH)2/H2O equal 4.11 and, Δwt is the weight loss in TGA curve due to the dehydration of portlandite.
It not possible to calculate the percentage of calcium hydrates (C-S-H, ettrin-gite and calcium aluminate hydrates) by the above method because calcium hy-drates has unknown structure and able to incorporate guest ions . Alterna-tively, it was assumed that the relative proportions of calcium hydrate species (C-S-H, ettringite and calcium aluminate and aluminosilicate hydrates) are the same for a particular cement paste under the same condition. Hence, the rate of dehydration of calcium hydrates in the fired cement pastes will be constant. Ac-cordingly, the approximate percentage of residual calcium hydrates in cement pastes fired at a given temperature relative to that in unfired cement paste can be estimated as follows:
Relative percentage of calcium hydrates (r) =(Δwtf/Δwt)× 100 Percentage of calcium hydrates decomposition = r − 100
where: Δwt is the weight loss in TGA curve corresponding to dehydration of cal-cium hydrates for unfired cement paste, and Δwtf is the weight loss correspond-ing to dehydration of calcium hydrates for cement paste fired at a given temper-ature.
3. Results and Discussion
Figure 2 illustrates the weight loss of cement pastes that were fired at 300˚C - 750˚C. Weight loss increases with temperature. Weight loss that occurs at 300˚C may be due to the evaporation of capillary water from macro capillary pores, evaporation of gel water from gel pores of cement paste and partial dehydration of C-S-H . Weight loss that occurs at 450˚C may be due to the dehydration of portlandite as evidenced from DTA results (Figure 3). Weight loss that occurs at 600˚C - 750˚C is due to the dehydration of residual portlandite and C-S-H as well as decomposition of calcite .
DOI: 10.4236/msce.2017.511004 38 Journal of Materials Science and Chemical Engineering
Figure 2. Weight loss of cement pastes fired at 300˚C - 750˚C.
Figure 3. DTA thermograms of cement pastes fired at 300˚C - 750˚C.
Figure 4. Bulk density and total porosity of cement pastes fired at 300˚C - 750˚C.
density leads to the suggestion that the hydration products that was formed un-der this hydrothermal condition have low density compared to that formed at ambient temperatures. With rising temperature above 300˚C, the decomposition of C-S-H and portlandite opens the pore system of cement paste and increases the total porosity .
Figure 5 illustrates the strength loss of cement paste fired at 300˚C - 750˚C. The loss in compressive strength may be considered as an important measure of
0 100 200 300 400 500 600 700 800 900 1000
300 ˚C 450 ˚C 600 ˚C 750 ˚C
DOI: 10.4236/msce.2017.511004 39 Journal of Materials Science and Chemical Engineering
Figure 5. Strength loss of cement pastes fired at 300˚C - 750˚C.
the degree of damage to concrete exposed to high temperatures. The streng-thening of unfired cement paste results from the coexistence of the amorphous and crystalline C-S-H that binds particles into cohesive mass . With rising temperature, a negligible and limited strength loss was observed at 300˚C and 450˚C then the strength loss markedly increases at the higher temperatures. This indicates that beyond the critical temperature of 450˚C the decomposition of C-S-H markedly progresses .
Figure 6 illustrates the FTIR spectra of cement paste fired at 300˚C - 750˚C. In the case of OPC, the wide band at around 923 - 930 cm−1, which is attributed to the ν3 (Si-O) asymmetric stretching vibrations of alite was shifted to higher wavenumbers (around 978 cm−1) as cement hydration progressed. In the case of the unfired cement sample, the formation of C-S-H gel was accompanied by a gradual weakening of the ν4 (O-Si-O) absorption band at 520 cm−1 which is at-tributed both to unhydrated alite and belite. The bands at 1144 and 1107 cm−1 which are attributed to ν3 asymmetric stretching vibrations of the sulfate group
SO−) in gypsum were replaced with a new band at around 1115 cm−1 that attribute to ν3 vibrations of 2
SO− in ettringite . In the case of fired cement pastes, the FTIR results can be utilized to monitor the phase changes due to ex-posure to high temperatures. Table 1 summarizes the relative intensity of the characteristic absorption bands given in Figure 6. C-S-H progressively decreases due to its decomposition above 450˚C. This agrees with the results of strength loss. C3S and C2S increase with rising temperature as a result of the decomposi-tion of C-S-H. Portlandite decreases due to its dehydradecomposi-tion around 450˚C. Trac-es of portlandite were detected at 600˚C - 750˚C due to the rehydration of lime . Calcite decomposes at 750˚C.
Figure 7 illustrates the TGA thermograms of cement paste fired at 300˚C - 750˚C. The first weight loss in the temperature range 25˚C - 320˚C is attributed to the dehydration of C-S-H, ettringite and calcium aluminate hydrates . The temperature at which these compounds lose water depends upon the CaO/SiO2 ratio in the hydrated cement matrix . The second and third weight loss in the temperature ranges 350˚C - 550˚C and 650˚C - 800˚C are attributed to the dehydration of portlandite and decarbonation of calcite respectively . A sig-nificant amount of calcite was detected in all of the hydrated samples is attri-buted to the limestone filler commonly added to OPC . The relative
0 10 20 30 40
300 450 600 750
DOI: 10.4236/msce.2017.511004 40 Journal of Materials Science and Chemical Engineering
Figure 6. FTIR spectra of cement pastes fired at 300˚C - 750˚C. (where: A alite, B belite, C calcite, E ettringite, G gypsum, P portlandite, W water), (vs very strong, s strong, m medium, w weak, - not found).
Figure 7. TGA thermograms of cement pastes fired at 300˚C - 750˚C.
percentage of residual portlandite and calcium hydrates in cement pastes fired at 300˚C - 750˚C are given in Table 2. These results give a crucial picture about the decomposition of amorphous calcium silicate hydrates which can not be de-tected by XRD analysis.
The percentage of portlandite that was estimated for the unfired cement paste (28.49%) nearly agrees with that typically reported in the literature (i.e. portlan-dite occupies 20% - 25% of the hydrated cement paste) . With rising tem-perature up to 300˚C, the percentage of portlandite slightly increases due to hy-dration of the OPC grains which was encouraged under the hydrothermal con-dition. Above 300˚C, the percentage of portlandite slightly diminishes due to dehydration of portlandite to lime. Whereas above 450˚C, the percentage of
W W C GE S A B
0 100 200 300 400 500 600 700 800 900 1000
Unfired 300 ˚C
DOI: 10.4236/msce.2017.511004 41 Journal of Materials Science and Chemical Engineering
Table 1. Relative intensity of characteristic absorption bands given in Figure 6.
Band, cm−1 Phase Relative intensity Reference
OPC Unfired 300˚C 450˚C 600˚C 750˚C
518 C2S (O-Si-O) Vs W s s s s 
937 C3S (Si-O) Vs W m m s s 
975 C-S-H (O-Si-O) - Vs s m - - 
1115 Ettringite ( 2 4
SO−) - M m m m m 
1144 Gypsum ( 2 4
SO−) Vs - - - 
1432 Calcite ( 2 3
CO−) Vs M s m m w 
1637, 3455 Free water (OH−) - S vs m w w 
3642 Portlandite (OH−) vw S vs m w w 
Table 2. The relative percentages of residual calcium hydrates and portlandite in cement pastes fired at 300˚C - 750˚C.
Unfired Calcium hydrates Portlandite Sample Mass change, % Decomposition percent, % Mass change, % Percent, % Unfired 5.13 - 6.93 28.49
300˚C 2.72 46.98 7.15 29.39 450˚C 2.38 53.61 5.05 20.76 600˚C 0.58 88.69 1.93 7.93 750˚C 0.23 95.52 1.30 5.34
portlandite sharply diminishes but does not fall to zero value in cement pastes that were fired at 600˚C - 750˚C due to the partial rehydration of lime. The per-centage of calcium hydrates was lowered to its half value with rising temperature up to 450˚C. A severe and complete loss of calcium hydrates content occurs when cement paste was subjected to 600˚C and 750˚C respectively. This con-firms that the dehydration of calcium hydrates is a multi-step reaction because of its complex structure  and occurs over a wide range temperature (i.e. from 105˚C to 1000˚C)  and . According to Jennings, the C-S-H gel consists of many small globules with a disordered layered structure, hence, water molecules release over a wide range temperature .
Figure 3 illustrates the DTA thermograms of cement paste fired at 300˚C - 750˚C. DTA results are useful to justify the dehydration process of portlandite. The endothermic peak located at about 450˚C in the case of unfired cement paste and that was fired at 300˚C - 450˚C corresponds to the dehydration of the primary portlandite that forms during the hydration of cement in the case of un-fired cement paste and remaining portlandite that present in cement paste un-fired up to 450˚C.
DOI: 10.4236/msce.2017.511004 42 Journal of Materials Science and Chemical Engineering the dehydration of the secondary portlandite that forms as a result of the rehy-dration of lime in the case of cement pastes fired above 450˚C. This result agrees with the previous results which illustrate that portlandite formed during the re-hydration of fired cement paste has an onset dere-hydration temperature lower than the original portlandite . The environments and formation condition of the primary and secondary portlandite is quite different, accordingly, their rate of dehydration are not equal. The secondary portlandite dehydrates at lower temperatures range may be due to the critical condition in which it forms which affect its surface area and particle size. The experimental results confirm that the decomposition of hydrates is affected by surface area and particle size .
Figure 8 illustrates the XRD patterns of cement pastes fired at 300˚C - 750˚C. The dominant crystalline phases that were detected in OPC are; alite, belite and calcite. The dominant crystalline phases that were detected in the unfired ce-ment paste are calcite filler and portlandite arising from the hydration process as well as small proportions of the unhydrated alite and belite. XRD patterns com-prise some changes in the phase compositions of cement paste with rising tem-perature. The proportion of portlandite diminishes above 450˚C . A signifi-cant proportion of belite and alite appears at 450˚C and progressively increases at 600˚C and 750˚C. This proves that the decomposition of C-S-H reaches a sig-nificant rate at 450˚C and enhances with rising temperature . This result agrees with FTIR and DTA results. According to Peng et al., it is difficult to dif-ferentiate between the peaks of C2S and C3S in XRD diagrams of cement pastes exposed to high temperatures. Hence, peaks of C2S and C3S can be used to
Figure 8. XRD patterns of cement pastes fired at 300˚C - 750˚C. (A alite, B belite, C cal-cite and P portlandite).
A B A
10 20 30 40 50 60
Unfired 300 ˚C
A B A P P P
DOI: 10.4236/msce.2017.511004 43 Journal of Materials Science and Chemical Engineering represent both of them . Figure 9 illustrates the SEM micrographs of cement paste fired at 300˚C - 750˚C. The results monitor the change in microstructure and phase compositions due to the hydration of OPC and the dehydration of cement paste fired at 300˚C - 750˚C. The micrograph of unfired cement shows OPC grains loaded with the hexagonal portlandite plates  and amorphous C-S-H formed during hydration of OPC. The microstructure of cement paste that was fired at 300˚C has not changed significantly. Whereas, some of unhy-drated cement grains and residues of hexagonal portlandite plates appear in the microstructure of cement paste that was fired at 450˚C. The micrograph of ce-ment paste that was fired at 600˚C shows the presence of distorted cubic calcite crystals . The micrograph of cement paste that was fired at 750˚C may show the presence of dehydration products. Accordingly, the decomposition of C-S-H significantly starts at 450˚C and progresses with rising temperature.
Figure 10 illustrates the crack propagation in cement paste fired at 300˚C - 750˚C. Minor cracks (about 0.1 mm in width) appeared on the surface of cement paste that was fired at 300˚C. The cracks widen and deepen with rising
Figure 9. SEM micrographs of cement pastes fired at 300˚C - 750˚C.
DOI: 10.4236/msce.2017.511004 44 Journal of Materials Science and Chemical Engineering
Figure 10. Crack propagation in cement paste fired at 300˚C - 750˚C.
temperature. Thin shallow linear superficial cracks (about 0.4 mm in width) ap-peared on the surface of cement paste that was fired at 450˚C. Thick grid-like deep cracks (about 0.8 mm in width) appeared on the surface of cement paste that was fired at 750˚C. The cracks form as a result of the following factors; 1) the internal pore pressure caused by water vapor that was accumulated after the dehydration of calcium hydrates in case of relatively low permeable cement paste accompanied by loss of mechanical strength, 2) the thermal shock that arises as a result of cooling of the heated cement paste, 3) the rehydration of lime that is accompanied by a significant volume increase .
FTIR, XRD, TGA/DTA and SEM techniques were used to monitor the micro-structural and compositional changes within cement paste induced with rising temperature. Accordingly, the main conclusions are:
1) The microstructure of cement paste that was fired at 300˚C has not changed significantly.
2) A negligible and limited strength loss was observed before 450˚C attributed to the dehydration of C-S-H, ettringite and calcium aluminate hydrates.
3) 450˚C is a critical temperature in the thermal damage history of cement paste, around which the percentage of portlandite decreases due to its dehydra-tion and the percentage of calcium hydrates was lowered to its half value.
4) Beyond 450˚C, the percentage of portlandite sharply diminishes and de-composition of C-S-H into C2S and C3S markedly progresses until complete loss of calcium hydrates content occurs at 750˚C.
5) These deleterious changes in the composition of cement paste are accom-panied by an increase of the total porosity, severe loss in mechanical strength
4 mm 4 mm
4 mm 4 mm
300 oC 450oC
DOI: 10.4236/msce.2017.511004 45 Journal of Materials Science and Chemical Engineering and propagation of harmful cracks.
6) The thermal shock that arises as a result of cooling of the heated cement paste and the rehydration of lime that is accompanied by a significant volume increase enhance the propagation of harmful cracks.
 Poon, C.S., Azhar, S., Anson, M. and Wong, Y.L. (2003) Performance of Metakaolin Concrete at Elevated Temperatures. Cement and Concrete Composites, 25, 83.  Khoury, G.A. (1992) Compressive Strength of Concrete at High Temperatures:
Reassessment. Magazine of Concrete Research, 44, 291.
 Jhang, K.Y. (2009) Non Linear Ultrasonic Techniques for Non Destructive Assess-ment of Micro Damage in Material: A Review. International Journal of Precision Engineering Manufacturing, 10, 123.https://doi.org/10.1007/s12541-009-0019-y  Park, S.J., Yim, H.J. and Kwak, H.G. (2014) Non Linear Resonance Vibration
Me-thod to Estimate the Damage Level on Heat-Exposed Concrete. Fire Safety Journal, 69, 36.
 Netinger, I., Varevac, D., Bjegovic, D. and Moric, D. (2013) Effect of High Temper-ature on Properties of Steel Slag Aggregate Concrete. Fire Safety Journal, 59, 1.  Ezziane, M., Kadri, T., Molez, L., Jauberthie, R. and Belhacen, A. (2015) High
Tem-perature Behavior of Polypropylene Fibers Reinforced Mortars. Fire Safety Journal, 71, 324.
 Ergun, A., Kurklu G., Baspınar, M.S. and Mansour, M.Y. (2013) The Effect of Ce-ment Dosage on Mechanical Properties of Concrete Exposed to High Temperatures. Fire Safety Journal, 55, 160.
 Reddy, D.V., Sobhan, K., Liu, L. and Young Jr, J.D. (2015) Size Effect on Fire Resis-tance of Structural Concrete. Engineering Structures, 99, 468.
 Xiao, J., Li, Z., Xie, Q. and Shen, L. (2016) Effect of Strain Rate on Compressive Be-havior of High-Strength Concrete after Exposure to Elevated Temperatures. Fire Safety Journal, 83, 25.
 Kontogeorgos, D.A., Semitelos, G.K., Mandilaras, I.D. and Founti, M.A. (2016) Ex-perimental Investigation of the Fire Resistance of Multi-Layer Drywall Systems In-corporating Vacuum Insulation Panels and Phase Change Materials. Fire Safety Journal, 81, 8.
 Wang, H.Y. (2008) The Effects of Elevated Temperature on Cement Paste Contain-ing GGBFS. Cement and Concrete Composites, 30, 992.
 Alonso, C. and Fernandez, L. (2004) Dehydration and Rehydration Processes of Cement Paste Exposed to High Temperature Environments, Materials Science, 39, 3015.https://doi.org/10.1023/B:JMSC.0000025827.65956.18
 Peng, G.F. and Huang, Z.S. (2008) Change in Microstructure of Hardened Cement Paste Subjected to Elevated Temperatures. Construction and Building Materials, 22, 593.
 Ai, H., Young, J.F. and Scherer, G.W. (2001) Thermal Expansion Kinetics: Method to Measure Permeability of Cementitious Materials: II, Application to Hardened Cement Pastes. Journal of the American Ceramic Society, 84, 385.
DOI: 10.4236/msce.2017.511004 46 Journal of Materials Science and Chemical Engineering of Polypropylene Fibres in Preventing Fire Spalling in Self-Compacting and High-Performance Cement Paste. Cement and Concrete Research, 38, 487.
 Xu, Y., Wong, Y.L., Poon, C.S. and Anson, M. (2003) Influence of PFA on Cracking of Concrete and Cement Paste after Exposure to High Temperatures. Cement and Concrete Research, 33, 2009.
 Heikal, M. (2000) Effect of Temperature on the Physico-Mechanical and Minera-logical Properties of Homra pozzolanic Cement Pastes. Cement and Concrete Re-search, 30, 1835.
 Morsy, M.M., Shebl, S.S. and Rashad, A.M. (2008) Effect of Fire on Microstructure and Mechanical Properties of Blended Cement Pastes Containing MK and SF. ASIAN Journal of Civil Engineering (Building and Housing), 9, 93.
 Rashad, A.M. and Zeedan, S.R. (2012) A Preliminary Study of Blended Pastes of Cement and Quartz Powder under the Effect of Elevated Temperature. Construc-tion and Building Materials, 29, 672.
 El-Didamony, H., Abd El-Rahman, E. and Osman, R.M. (2012) Fire Resistance of Fired Clay Bricks-Fly Ash Composite Cement Pastes. Ceramics International, 38, 201.
 Morsy, M.S., Galal, A.F. and Abo-EI-Enein, S.A. (1998) Effect of Temperature on Phase Composition and Microstructure of Artificial Pozzolana-Cement Pastes Containing Burnt Kaolinite Clay. Cement and Concrete Research, 28, 1157.
 Tantawy, M.A., El-Roudi, A.M., Abdalla, E.M. and Abdelzaher, M.A. (2013) Fire Resistance of Sewage Sludge Ash Blended Cement Pastes. Journal of Engineering.  Stepkowska, E.T., Blanes, J.M., Franco, F., Real, C. and Pérez-Rodriguez, J.L. (2004)
Phase Transformation on Heating of an Aged Cement Paste. Thermochimica Acta, 420, 79.
 Heikal, M. (2006) Effect of Temperature on the Structure and Strength Properties of Cement Pastes Containing Fly Ash Alone or in Combination with Limestone. Ce-ramics Silikaty, 50, 167.
 Alarcon-Ruiz, L., Platret, G., Massieu, E. and Ehrlacher, A. (2005) The Use of Thermal Analysis in Assessing the Effect of Temperature on a Cement Paste. Ce-ment and Concrete Research, 35, 609.
 Ukrainczyk, N., Ukrainczyk, M., Šipušić, J. and Matusinović, T. (2006) XRD and TGA Investigation of Hardened Cement Paste Degradation. 11th Conference on Materials, Processes, Friction and Wear, Vela Luka.
 Ye, G., Liu, X., De Schutter, G., Taerwe, L. and Vandevelde, P. (2007) Phase Distri-bution and Microstructural Changes of Self-Compacting Cement Paste at Elevated Temperature. Cement and Concrete Research, 37, 978.
 Zhang, Q. and Ye, G. (2012) Dehydration Kinetics of Portland Cement Paste at High Temperature. Journal of Thermal Analysis and Calorimetry, 110, 153.
 Khoury, G.A., Majorana, C.E., Pesavento, F. and Schrefler, B.A. (2002) Modeling of Heated Concrete. Magazine of Concrete Research, 54, 77.
 Rehsi, S.S. (1993) Portland Fly Ash Cement in Mineral Admixtures in Cement and Concrete. Edited by Ghosh, S.N., Sarkar, S.L., and Harsh, S., ABI Books, New Delhi, 158.
Com-DOI: 10.4236/msce.2017.511004 47 Journal of Materials Science and Chemical Engineering posites, 34, 1067.
 Maaroufi, M.A., Lecomte, A., Diliberto, C., Francy, O. and Brun, P. (2015) Ther-mo-Hydrous Behavior of Hardened Cement Paste Based on Calcium Aluminate Cement. European Ceramic Society, 35, 1637.
 Vysvaril, M., Bayer, P., Chroma, M. and Rovnanikova, P. (2014) Physi-co-Mechanical and Microstructural Properties of Rehydrated Blended Cement Pastes. Construction and Building Materials, 54, 413.
 Lin, W.M., Lin, T.D. and Powers-Couche, L.J. (1996) Microstructures of Fire Dam-aged Concrete. ACI Materials, 93, 199.
 Poon, C.S., Azhar, S., Anson, M. and Wong, Y. (2001) Strength and Durability Re-covery of Fire Damaged Concrete after Post-Fire-Curing. Cement and Concrete Research, 30, 1307.
 Shui, Z., Xuan, D., Wan, H. and Cao, B. (2008) Rehydration Reactivity of Recycled Mortar from Concrete Waste Experienced to Thermal Treatment. Construction and Building Materials, 22, 1723.
 Serpell, R. and Lopez, M. (2013) Reactivated Cementitious Materials from Hydrated Cement Paste Wastes. Cement and Concrete Composites, 39, 104.
 ASTM Designation (1983) C109-80, Standard Test Methods for Compressive Strength of Hydraulic Cements. Annual Book of ASTM Standards.
 Kumar, S. and Kameswara Rao, C.V.S. (1995) Strength Loss in Concrete Due to Varying Sulfate Exposures. Cement and Concrete Research, 25, 57.
 Pavlik, J., Tydlitat, V., Cerny, R., Klecka, T., Bouska, P. and Rovnanikova, P. (2003) Application of a Microwave Impulse Technique to the Measurement of Free Water Content in Early Hydration Stages of Cement Paste. Cement and Concrete Re-search, 33, 93.
 Gennaro, R., Cappelletti, P., Cerri, G., Gennaro, M., Dondi, M. and Langella, A. (2004) Zeolitic Tuffs as Raw Materials for Lightweight Aggregates. Applied Clay Science, 25, 71.
 Copeland, L.E. and Hayes, T.C. (1956) Porosity of Hardened Portland Cement Pastes. American Concrete Institute, Materials, 27, 633.
 ISO (1983) 5018:1983, Determination of True Density of Refractory and Other Raw Materials.
 Földvári, M. (2011) Handbook of Thermogravimetric System of Minerals and Its Use in Geological Practice. Geological Institute of Hungary, Budapest.
 Dolado, J.S., Griebe, M. and Hamaekers, J. (2007) A Molecular Dynamic Study of Cementitious Calcium Silicate Hydrate (C-S-H) Gels. Journal of the American Ce-ramics Society, 90, 3938.
 Zhang, B. (2011) Effects of Moisture Evaporation (Weight Loss) on Fracture Prop-erties of High Performance Concrete Subjected to High Temperatures. Fire Safety Journal, 46, 543.
 Saad, M., Abo-El-Enein, S.A., Hanna, G.B. and Kotkata, M.F. (1996) Effect of Tem-perature on Physical and Mechanical Properties of Concrete Containing Silica Fume. Cement and Concrete Research, 26, 669.
 Rashad, A.M., Sadek, D.M. and Hassan, H.A. (2016) An Investigation on Blast-Furnace Slag as Fine Aggregate in Alkali Activated Slag Mortars Subjected to Elevated Temperatures. Journal of Cleaner Production, 112, 1086.
DOI: 10.4236/msce.2017.511004 48 Journal of Materials Science and Chemical Engineering Admixtures on Calcium Aluminate Cement Pastes. Part 2: Hydration Studies. In-dustrial and Engineering Chemistry Research, 52, 17330.
 Matossi, F. (1949) Vibration Frequencies and Binding Forces in Some Silicate Groups. Journal of Chemical Physics, 17, 679. https://doi.org/10.1063/1.1747369  Bakharev, T. (2005) Geopolymeric Materials Prepared using Class F Fly Ash and
Elevated Temperature Curing. Cement and Concrete Research, 35, 1224.
 Gadsden, J.A. (1975) Infrared Spectra of Minerals and Related Inorganic Com-pounds. 3rd Edition, Butterworths, London.
 Liew, Y.M., Kamarudin, H., Mustafa Al Bakri, A.M., Luqman, M., Khairul Nizar, I., Ruzaidi, C.M. and Heah, C.Y. (2012) Processing and Characterization of Calcined Kaolin Cement Powder. Construction and Building Materials, 30, 794.
 Vedalakshmi, R., Sundara Raj, A., Srinivasan, S. and Ganesh Babu, K. (2003) Quan-tification of Hydrated Cement Products of Blended Cements in Low and Medium Strength Concrete using TG and DTA Technique. Thermochimica Acta, 407, 49.  Mitchell, L.D. and Margeson, J.C. (2006) The Effect of Solvents on C-S-H as
Deter-mined by Thermal Analysis. Journal of Thermal Analysis and Calorimetry, 86, 591.  European Committee for Standardization (2000) Cement: Common Cements. PrEN
197-1, CEN/TC51/WG 6 rev., Final Draft.
 Mobasher, B. (2002) Hydration, Best 50 Minutes, Undergraduate Faculty Develop-ment. NSF Center for Advanced Cement Based Materials, Northwestern University.  Jennings, H.M. (2008) Refinements to Colloid Model of C-S-H in Cement: CM-II.
Cement and Concrete Research, 38, 275.
 Boynton, R.S. (1980) Chemistry and Technology of Lime and Limestone. John Wi-ley and Sons, New York.
 Platret, G. (2002) Monitoring the Hydration of Cement and the Evolution of Solid Phases in Concrete by Thermal Analysis. Microstructural Characteristics and Prop-erties Related to the Durability of Concrete. Methods of Measuring and Testing La-boratory, Test Methods No. 58, Central Laboratory of Bridges and Roads, Paris.  Mehta, P.K. (1986) Concrete, Structure, Properties and Materials. Prentice-Hall,
Englewood Cliffs, 450.
 Wang, H., Alfredsson, V., Tropsch, J., Ettl, R. and Nylander, T. (2013) Formation of CaCO3 Deposits on Hard Surfaces: Effect of Bulk Solution Conditions and Surface Properties. ACS Applied Material Interfaces, 5, 4035.